# Imperfection Sensitivity of Nonlinear Vibration of Curved Single-Walled Carbon Nanotubes Based on Nonlocal Timoshenko Beam Theory

^{1}

^{2}

^{3}

^{4}

^{5}

^{*}

## Abstract

**:**

## 1. Introduction

## 2. Problem Formulation

#### 2.1. Timoshenko Beam Model for Vibration of Curved Single-Walled Carbon Nanotubes (SWCNTs)

#### 2.2. Nonlocal Theory of Nano-Beams

#### 2.3. Derivation of Nonlocal Governing Equations of Motion

#### 2.4. Differential Quadrature Solution Procedure

## 3. Numerical Results and Discussions

#### 3.1. Results Verification

_{s}= 0.563 [37]. As expected, increasing the nonlocal effect causes a decrease in dimensionless frequency. A noteworthy agreement is observed between the present results and those reported by Yang et al. [22]. Good agreement is observed between the results of current study and those by Wang et al. [37]. However, because they neglected the nonlocal terms in shearing force relation, the discrepancy between the results of two methods increases for higher values of nonlocal parameter.

_{s}= 0.563. Nonlocal parameter, $\mu $, and nonlinear vibration amplitude, ${w}_{max}^{*}$, are set to 0.15 and 0.4, respectively. For both linear and nonlinear frequencies, good agreement exists between the results of current study and those reported in [22].

#### 3.2. Geometric Imperfection Function

_{1}” to “L

_{3}” types. It is seen that the imperfection is exactly located at the center of SWCNT for L

_{3}type while for the L

_{1}type the imperfection is the closest case to the end.

#### 3.3. Nonlinear Vibration of Curved SWCNTs

_{1},” “L

_{2}” and “L

_{3}” are local imperfections with maximum amplitude of η = 0.1. For all local imperfect cases, the hard-spring behavior is observed. It is seen that the local imperfection has the largest effect on the nonlinear frequency ratio when it is located in the center of the single-walled carbon nanotube (L

_{3}) and its effect is decreased when the imperfection recedes from the center to the boundary (L

_{1}).

_{3}” is selected as the geometric imperfection with maximum amplitude of η = 0.1. Unlike straight SWCNTs (perfect case), curved nanotubes (imperfect cases) do not have an overall increasing trend for nonlinear frequency ratio while the nonlocal parameter μ raises, and there is a certain value of amplitude vibration ${w}_{max}^{*}$ in which the effect of nonlocal parameter gets reversed. Furthermore, it is observed that SWCNTs with C–C boundary condition have the highest nonlinear frequency and the H–H SWCNTs have the lowest, as expected.

_{2}) geometry is illustrated in Figure 8. Like the “G” type imperfection, the imperfection sensitivity ${S}_{w}$ increases when the maximum imperfection amplitude η is raised. For small values of imperfection amplitude η, all values of the nonlocal parameter almost have the same behavior, but after a certain value of η, a sudden large increase in imperfection sensitivity value occurs for higher values of nonlocal parameter μ. It depicts that for the case of local imperfection with large values of nonlocal parameter, initial geometric imperfections may cause considerable change in the fundamental frequency which cannot be neglected.

## 4. Conclusions

## Acknowledgments

## Author Contributions

## Conflicts of Interest

## Abbreviations

CNTs | Carbon Nano Tubes |

DQ | Differential Quadrature |

MD | Molecular Dynamics |

NEMS | Nano Electro Mechanical System |

SWCNTs | Single-Walled Carbon Nano Tubes |

## References

- Bosia, F.; Lepore, E.; Alvarez, N.T.; Miller, P.; Shanov, V.; Pugno, N. Knotted synthetic polymer or carbon nanotube microfibres with enhanced toughness, up to 1400 J/g. Carbon
**2016**, 102, 116–125. [Google Scholar] [CrossRef] - Ke, C.H.; Pugno, N.; Peng, B.; Espinosa, H.D. Experiments and modeling of carbon nanotube-based NEMS devices. J. Mech. Phys. Solids
**2005**, 53, 1314–1333. [Google Scholar] [CrossRef] - Ke, C.H.; Espinosa, H.D.; Pugno, N. Numerical analysis of nanotubes based NEMS devices—Part II: Role of finite kinematics, stretching and charge concentrations. J. Appl. Mech.
**2005**, 72, 519–526. [Google Scholar] [CrossRef] - Hierold, C.H.; Jungen, A.; Stampfer, C.H.; Helbling, T.H. Nano electromechanical sensors based on carbon nanotubes. Sens. Actuators A Phys.
**2007**, 136, 51–61. [Google Scholar] [CrossRef] - Liew, K.M.; Wang, Q. Analysis of wave propagation in carbon nanotubes via elastic shell theories. Int. J. Eng. Sci.
**2007**, 45, 227–241. [Google Scholar] [CrossRef] - Strozzi, M.; Smirnov, V.V.; Manevitch, L.I.; Milani, M.; Pellicano, F. Nonlinear vibrations and energy exchange of single-walled carbon nanotubes. Circumferential flexural modes. J. Sound Vib.
**2016**, 381, 156–178. [Google Scholar] [CrossRef] - Wang, C.Y.; Ru, C.Q.; Mioduchowski, A. Applicability and limitations of simplified elastic shell equations for carbon nanotubes. J. Appl. Mech.
**2004**, 71, 622–631. [Google Scholar] [CrossRef] - Smirnov, V.V.; Manevitch, L.I.; Strozzi, M.; Pellicano, F. Nonlinear optical vibrations of single-walled carbon nanotubes, Energy exchange and localization of low-frequency oscillations. Physica D
**2016**, 325, 113–125. [Google Scholar] [CrossRef] - Silvestre, N.; Wang, C.M.; Zhang, Y.Y.; Xiang, Y. Sanders shell model for buckling of single-walled carbon nanotubes with small aspect ratio. Compos. Struct.
**2011**, 93, 1683–1691. [Google Scholar] [CrossRef] - Amabili, M. A comparison of shell theories for large-amplitude vibration of circular cylindrical shells: Lagrangian approach. J. Sound Vib.
**2003**, 264, 1091–1125. [Google Scholar] [CrossRef] - Gibson, R.F.; Ayorinde, O.E.; Wen, Y.F. Vibration of carbon nanotubes and there composites: A review. Compos. Sci. Technol.
**2007**, 67, 1–28. [Google Scholar] [CrossRef] - Eringen, A.C. Nonlocal Continuum Field Theories; Springer: New York, NY, USA, 2002. [Google Scholar]
- Barretta, R.; Feo, L.; Luciano, R.; Marotti de Sciarra, F. An Eringen-like model for Timoshenko nanobeams. Compos. Struct.
**2016**, 139, 104–110. [Google Scholar] [CrossRef] - Barretta, R.; Feo, L.; Luciano, R.; Marotti de Sciarra, F.; Penna, R. Functionally graded Timoshenko nanobeams: A novel nonlocal gradient formulation. Compos. B
**2016**, 100, 208–219. [Google Scholar] [CrossRef] - Čanadija, M.; Barretta, R.; Marotti de Sciarra, F. On functionally graded Timoshenko nonisothermal nanobeams. Compos. Struct.
**2016**, 135, 286–296. [Google Scholar] [CrossRef] - Wang, Q.; Varadan, V.K. Wave characteristics of carbon nanotubes. Int. J. Solids Struct.
**2006**, 43, 254–265. [Google Scholar] [CrossRef] - Lu, P.; Lee, H.P.; Lu, C.; Zhang, P.Q. Application of nonlocal beam models for carbon nanotubes. Int. J. Solids Struct.
**2007**, 44, 5289–5300. [Google Scholar] [CrossRef] - Murmu, T.; Pradhan, S.C. Thermo-mechanical vibration of a single-walled carbon nanotube embedded in an elastic medium based on nonlocal elasticity theory. Comput. Mater. Sci.
**2009**, 46, 854–859. [Google Scholar] [CrossRef] - Ansari, R.; Sahmani, S. Small scale effect on vibrational response of single-walled carbon nanotubes with different boundary conditions based on nonlocal beam models. Commun. Nonlinear Sci.
**2012**, 17, 1965–1979. [Google Scholar] [CrossRef] - Reddy, J.N. Nonlocal nonlinear formulations for bending of classical and shear deformation theories of beams and plates. Int. J. Eng. Sci.
**2010**, 48, 1507–1518. [Google Scholar] [CrossRef] - Reddy, J.N. Nonlocal theories for bending, buckling, and vibration of beams. Int. J. Eng. Sci.
**2007**, 45, 288–307. [Google Scholar] [CrossRef] - Yang, J.; Ke, L.L.; Kitipornchai, S. Nonlinear free vibration of single-walled carbon nanotubes using nonlocal Timoshenko beam theory. Physica E
**2010**, 42, 1727–1735. [Google Scholar] [CrossRef] - Fang, B.; Zhen, Y.; Zhang, C.; Tang, Y. Nonlinear vibration analysis of double-walled carbon nanotubes based on nonlocal elasticity theory. Appl. Math. Model.
**2013**, 37, 1096–1107. [Google Scholar] [CrossRef] - Kitipornchai, S.; Yang, J.; Liew, K.M. Semi-analytical solution for nonlinear vibration of laminated FGM plates with geometric imperfections. Int. J. Solids Struct.
**2004**, 41, 2235–2257. [Google Scholar] [CrossRef] - Yamaki, N.; Otomo, K.; Chiba, M. Nonlinear vibrations of a clamped rectangular plate with initial deflection and initial edge displacement-Part 2: Experiment. Thin. Walled Struct.
**1983**, 1, 101–109. [Google Scholar] [CrossRef] - Calabri, L.; Pugno, N.; Ding, W.; Ruoff, R. Resonance of curved nanowires. J. Phys. Condens. Matter
**2006**, 18, S2175–S2183. [Google Scholar] [CrossRef] - Farshidianfar, A.; Soltani, P. Nonlinear flow-induced vibration of a SWCNT with a geometrical imperfection. Comput. Mater. Sci.
**2012**, 53, 105–116. [Google Scholar] [CrossRef] - Ouakad, H.M.; Younis, M.I. Natural frequencies and mode shapes of initially curved carbon nanotube resonators under electric excitation. J. Sound Vib.
**2011**, 330, 3182–3195. [Google Scholar] [CrossRef] - Amabili, M. Nonlinear vibrations of rectangular plates with different boundary conditions: Theory and experiments. Comput. Struct.
**2004**, 82, 2587–2605. [Google Scholar] [CrossRef] - Eringen, A.C. On differential equations of nonlocal elasticity and solutions of screw dislocation and surface waves. J. Appl. Phys.
**1983**, 54, 4703–4710. [Google Scholar] [CrossRef] - Jalali, S.K.; Rastgoo, A.; Eshraghi, I. Large amplitude vibration of imperfect shear deformable nano-plates using non-local theory. J. Solid Mech.
**2011**, 3, 64–73. [Google Scholar] - Pradhan, S.C.; Murmu, T. Small Scale Effect on the Buckling of Single-Layered Graphene Sheets under Bi-axial Compression via Nonlocal Continuum Mechanics. Comput. Mater. Sci.
**2009**, 47, 268–274. [Google Scholar] [CrossRef] - Shu, C. Differential Quadrature and Its Application in Engineering; Springer: London, UK, 2000. [Google Scholar]
- Malekzadeh, P.; Vosoughi, A.R. DQM large amplitude vibration of composite beams on nonlinear elastic foundations with restrained edges. Commun. Nonlinear Sci.
**2009**, 14, 906–915. [Google Scholar] [CrossRef] - Bhasyam, G.R.; Prathap, G. Galerkin finite element method for non-linear beam vibrations. J. Sound Vib.
**1980**, 72, 191–203. [Google Scholar] [CrossRef] - Marur, S.R.; Prathap, G. Non-linear beam vibration problems and simplifications in finite element models. Comput. Mech.
**2005**, 35, 352–360. [Google Scholar] [CrossRef] - Wang, C.M.; Zhang, Y.Y.; He, X.Q. Vibration of nonlocal Timoshenko beams. Nanotechnology
**2007**, 18, 105401. [Google Scholar] [CrossRef]

**Figure 4.**Variation of nonlinear vibration frequency ratio for different combinations of imperfection amplitude η and nonlocal parameter μ for a “G” type imperfection for (

**a**) clamped-clamped (

**b**) clamped-hinged and (

**c**) hinged-hinged endpoint conditions.

**Figure 5.**Variation of nonlinear vibration frequency ratio for (

**a**) clamped-clamped and (

**b**) hinged-hinged endpoint conditions of a nonlocal nano-beam for various “L” types imperfection.

**Figure 6.**Effects of nonlocal parameter μ on the nonlinear vibration frequency ratio of nano-beam with “L

_{3}” type of initial imperfection.

**Figure 7.**Effect of nonlocal parameter μ on sensitivity indicator of a nano-beam with “G” type initial imperfection with hinged-hinged endpoint conditions.

**Figure 8.**Effect of nonlocal parameter μ on sensitivity indicator of a nano-beam with “L

_{2}” type initial imperfection for (

**a**) clamped-clamped (

**b**) clamped-hinged and (

**c**) hinged-hinged endpoint conditions.

**Table 1.**Comparison of nonlinear frequency ratio of a Timoshenko straight beam for different vibration amplitudes.

$\frac{{\mathit{w}}_{\mathbf{\text{max}}}}{\sqrt{{\mathit{I}}_{\mathbf{2}}\mathbf{/}\mathcal{A}}}$ | H–H | C–C | C–H | ||||||
---|---|---|---|---|---|---|---|---|---|

Ref. [35] | Ref. [36] | Present | Ref. [35] | Ref. [36] | Present | Ref. [35] | Ref. [36] | Present | |

1.0 | 1.118 | 1.118 | 1.1181 | 1.0295 | 1.0283 | 1.0295 | 1.0641 | 1.0582 | 1.0593 |

2.0 | 1.4141 | 1.4135 | 1.4143 | 1.1127 | 1.1105 | 1.1128 | 1.2318 | 1.215 | 1.2182 |

3.0 | 1.8026 | 1.8027 | 1.8029 | 1.2377 | 1.2336 | 1.2378 | 1.4603 | 1.4368 | 1.4416 |

4.0 | 2.2359 | 2.2361 | 2.2363 | 1.3920 | 1.3856 | 1.3921 | 1.7210 | 1.6822 | 1.7026 |

5.0 | 2.6923 | 2.6925 | 2.6928 | 1.5659 | 1.5574 | 1.5660 | 1.9995 | 1.9180 | 1.9862 |

**Table 2.**Comparison of dimensionless linear frequency ($\omega {l}^{2}\sqrt{\rho \mathcal{A}/E{I}_{2}}$) of a straight nano-beam with different nonlocal parameter µ and various endpoint conditions.

μ | H–H | C–C | C–H | ||||||
---|---|---|---|---|---|---|---|---|---|

Ref. [37] | Ref. [22] | Present | Ref. [37] | Ref. [22] | Present | Ref. [37] | Ref. [22] | Present | |

0.0 | 3.0929 | – | 3.0929 | 4.4491 | – | 4.4491 | 3.7845 | – | 3.7844 |

0.1 | 3.0243 | 3.0210 | 3.0210 | 4.3471 | 4.3269 | 4.3269 | 3.6939 | 3.6849 | 3.6849 |

0.3 | 2.6538 | 2.6385 | 2.6385 | 3.7895 | 3.7032 | 3.7032 | 3.2115 | 3.1724 | 3.1724 |

0.5 | 2.2867 | 2.2665 | 2.2665 | 3.2420 | 3.1372 | 3.1371 | 2.7471 | 2.6982 | 2.6980 |

0.7 | 2.0106 | – | 1.9899 | 2.8383 | – | 2.7327 | 2.4059 | – | 2.3569 |

**Table 3.**Comparison of linear and nonlinear dimensionless frequency of a straight nonlocal nano-beam with μ = 0.15 and ${w}_{max}^{*}=0.4$.

Frequency | H–H | C–C | C–H | |||
---|---|---|---|---|---|---|

Ref. [22] | Present | Ref. [22] | Present | Ref. [22] | Present | |

${\omega}_{l}^{*}$ | 0.4233 | 0.4233 | 0.8055 | 0.8055 | 0.6052 | 0.6052 |

${\omega}_{nl}^{*}$ | 0.4405 | 0.4435 | 0.8188 | 0.8219 | 0.6197 | 0.6236 |

© 2016 by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC-BY) license (http://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Eshraghi, I.; Jalali, S.K.; Pugno, N.M. Imperfection Sensitivity of Nonlinear Vibration of Curved Single-Walled Carbon Nanotubes Based on Nonlocal Timoshenko Beam Theory. *Materials* **2016**, *9*, 786.
https://doi.org/10.3390/ma9090786

**AMA Style**

Eshraghi I, Jalali SK, Pugno NM. Imperfection Sensitivity of Nonlinear Vibration of Curved Single-Walled Carbon Nanotubes Based on Nonlocal Timoshenko Beam Theory. *Materials*. 2016; 9(9):786.
https://doi.org/10.3390/ma9090786

**Chicago/Turabian Style**

Eshraghi, Iman, Seyed K. Jalali, and Nicola Maria Pugno. 2016. "Imperfection Sensitivity of Nonlinear Vibration of Curved Single-Walled Carbon Nanotubes Based on Nonlocal Timoshenko Beam Theory" *Materials* 9, no. 9: 786.
https://doi.org/10.3390/ma9090786